F E A T U R E A R T I C L E
Hexagonal boron nitride on transition metal surfacesJaime Go´mez Dı´az•Yun Ding• Ralph Koitz•
Ari P. Seitsonen•Marcella Iannuzzi•
Received: 31 October 2012 / Accepted: 1 February 2013 / Published online: 27 February 2013 Ó The Author(s) 2013. This article is published with open access at Springerlink.com
Abstract We validate a computational setup based on density functional theory to investigate hexagonal boron nitride (h-BN) monolayers grown on different transition metals exposing hexagonal surfaces. An extended assessment of our approach for the characterization of the geometrical and electronic structure of such systems is performed. Due to the lattice mismatch with the substrate, the monolayers can form Moire´-type superstructures with very long periodicities on the surface. Thus, proper models of these interfaces require very large simulation cells (more than 1,000 atoms) and an accurate description of interactions that are modulated with the specific registry of h-BN on the metal. We demonstrate that efficient and accurate calculations can be performed in such large systems using Gaussian basis sets and dispersion corrections to the (semi-)local density functionals. Four different metallic substrates, Rh(111), Ru(0001), Cu(111), and Ni(111), are explicitly considered, and the results are compared with pre-vious experimental and computational studies.
Keywords Density functional theory Nanomesh Boron nitride Interfaces Metal surfaces
Precise positioning and the control of interactions of indi-vidual molecules or small assemblies of atoms are of prime importance in the field of nano-devices. A promising way
to obtain well-defined arrangements on a large scale is through template surfaces. These show a variation of the interaction strength on a nanometer scale. Optimally, the template will not interact too strongly with the nanostruc-tures and should affect only weakly their electronic prop-erties. Such functionalized surfaces have many possible applications in chemistry and biology and are essential in nano-electronics.
Monolayers of hexagonal boron nitride (h-BN) , as well as the isoelectronic carbon structure, graphene (gr), grown on transition metal (TM) surfaces have received much interest as possible templates for use in nano-devices. Chemical vapour deposition of precursor molecules, e.g., borazine in the case of h-BN, on a hot metallic surface leads to a spontaneous formation of the uniform epitaxial monolayers. Originally, the preparation of a single layer of h-BN was achieved on the Rh(111) surface [1, 2], but recently similar structures have been grown on Ru(0001) [3–5], Pt(111) [4, 6, 7], Ni(111) [8–10], Cu(111) , Pd(111) , and Ag(111) . One-dimensional struc-tures of h-BN have been produced using the same proce-dure on Cr(110) , Fe(110) , and Mo(110) . Using similar recipes, graphene structures on most of these TM surfaces have also been obtained [5,16].
As the monolayer is adsorbed, its properties can become periodically modulated to form an extended superstructure. An important motivation of this work is to investigate the properties of such superstructures and the conditions under which they can be obtained. The long-range structure of the monolayer depends strongly on a series of factors: the mismatch a in the unit cell length l of the free-standing monolayer and the TM surface,
a¼lBN lTM lTM
; J. Go´mez Dı´az: Deceased.
J. Go´mez Dı´az Y. Ding R. Koitz A. P. Seitsonen M. Iannuzzi J. Hutter (&)
Physical Chemistry Institute, University of Zu¨rich, Winterthurerstrasse 190, 8057 Zurich, Switzerland e-mail: Hutter@pci.uzh.ch
the distance-dependence of the h-BN to metal interaction, and the deformation energy, both in- and out-of-plane, of the monolayer. In h-BN/Rh(111), the balance between lattice mismatch a of -7.0 % and quite strong rhodium– nitrogen interaction leads to a strongly corrugated structure with a periodicity of 3.22 nm, the so-called nanomesh . The highly regular hexagonal arrangement corresponds to a coincidence lattice of 13 9 13 h-BN on 12 9 12 Rh unit cells. The adsorbate is characterized by ‘‘pores’’ of about 2 nm diameter that strongly interact with the metal and elevated regions, where the interaction with the metal is weak, that form the connected ‘‘wire’’ network. The strong variation in bonding leads to a corresponding variation of the electrostatic potential above the monolayer that is responsible for trapping molecules . The h-BN/ Rh(111) nanomesh is a very stable structure that withstands temperatures of 1,000 K and can be exposed to liquids without losing its properties. Reversibility of the modification of the structure using atomic hydrogen has also been demonstrated . Similar nanomesh structures have been found on Ru(0001), Pd(111), and Pt(111), which present comparable or even larger lattice constant mismatches. On other metals, like Ag, with a weak interaction and smaller differences in the lattice constants, commensurate structures with no preferred relative orientation [9,12] have been observed.
Density functional theory (DFT)-based electronic structure calculations have been instrumental in the understanding of the structure and properties of the h-BN and gr nanomeshes [2,5,12,17, 19]. Experimental tech-niques applied to characterize the nanomesh, i.e., scanning tunnelling microscopy (STM) and spectroscopy (STS), surface X-ray diffraction (SXRD), ultraviolet (UV), and X-ray photoemission spectroscopy (UPS, XPS), as well as X-ray absorption spectroscopy (XAS), all profit in inter-pretation from independent simulations. Previous simula-tions primarily used DFT with the generalized gradient approximation (GGA) and either the linearized augmented plane wave (LAPW) method [19–24] or a plane wave (PW) basis set [25–28].
We have developed an approach to investigate na-nomeshes based on the Gaussian and plane wave (GPW)  formalism: A localized Gaussian basis positioned at each atom is used to expand the Kohn–Sham orbitals and a PW basis to describe the electron density to facilitate the calculation of the Coulomb interactions. This formalism leads to a very efficient description of the orbitals that can make use of locality in large systems and at the same time allows for the solution of the Poisson equation within linear time (in system size) . By adding an empirical pair potential to account for long-range van der Waals (vdW) forces [31,32] to a carefully chosen GGA functional, we achieve a balanced description of all important parts of the
system energy. We will first show that the chosen model parameters give a faithful description of important prop-erties of the individual systems, namely bulk and surfaces of metals and h-BN. We will then characterize four h-BN/ TM systems (TM: Rh, Ru, Cu, and Ni), thereby also pro-viding an overview of earlier calculations and experimental data.
2 Computational details and methods of analysis Calculations are performed using Kohn–Sham DFT [33, 34] within the GPW formalism as implemented in the Quickstep module in the CP2K program package . Dual-space pseudopotentials [36–38] are used to describe the interaction of valence electrons with atomic cores. The pseudopotentials for boron and nitrogen assume 3 and 5 valence electrons, respectively. The atomic cores of the metals are described by either a large- or medium-size core pseudopotential. In particular, for Rh we use potentials with 9 or 17 explicit valence electrons (q9, q17), for Ru 8 or 16 (q8, q16), 18 for Ni (q18), and 11 for Cu (q11). The PW energy cutoff for the expansion of the density is set at 500 Ry. If not stated otherwise, the Brillouin zone is sampled only at the C point. Exchange and correlation contributions are calculated with the Perdew-Burke-Ern-zerhof (PBE) [39, 40] and revised PBE (revPBE)  GGA exchange-correlation (XC) functionals. The latter is used together with the corrections for the long-range dis-persion interactions, computed using either the DFT-D2  or DFT-D3 formalisms , that are missing in GGA’s. The XC functional and its derivative are calculated on the same uniform density grid that is used for the Hartree energy and defined by the choice of the PW energy cutoff. In order to improve the accuracy and reduce numerical noise in the evaluation of the XC terms, a nearest neighbour smoothing procedure is employed. More details about these techniques are illustrated in Ref. . The Fermi–Dirac smearing of occupation numbers with a 300 K electronic temperature is used in all calculations. Broyden density mixing  is used to facilitate smooth convergence within a reasonable number of iterations. Periodic boundary conditions are applied in all calcula-tions. In calculations with slab-like models, interactions with periodic images in the direction perpendicular to the exposed surface are avoided by adding about 20 A˚ of vacuum space above the slab.
The optimized structures of h-BN on the different metallic substrates are characterized in terms of structural parameters, like buckling bBN (height difference of
neighbouring B and N), global corrugation DhB;N
(min-to-max height difference of B and N sublattices, respectively) and minimum distance of B or N from the TM dmin(B, N).
The strength of the interaction between TM and h-BN is evaluated as
Eint¼ Etot ðE f slabþ E f hBNÞ h i =NBN: ð1Þ
where Etot is the energy of the full system, Eslabf and
Eh-BNf are the energies of metallic slab and h-BN overlayer,
respectively, considered individually and with the same coordinates as in the full system (without relaxing them), and NBNis the number of the BN pairs in the full system.
The adsorption energy Eads¼ Etot ðEoslabþ E
is, instead, calculated with respect to the optimized free-standing h-BN and the optimized bare metallic slab.
The effects on the electronic structure due to the interac-tion between the TM and h-BN is investigated by the cal-culation of charge density differences between the full systems and its constituents (slab and h-BN) at the geometry of the combined system. The density of states projected on selected subsets of atoms (PDOS) and the representation of the electronic structure through maximally localized Wannier functions (MLWF)  are also useful descriptors of the electronic structure properties. The Tersoff-Hamann approximation [44,45] in STM simulations is used to yield the iso-current topography above the nanomesh. Given a bias potential Vb(often a fraction of eV), we determine the
iso-current surface as the set of grid points where nbðzÞe2kR0
¼ const. ð3Þ
In this expression, z is the height above the slab, nb the
electron density due to the states with energies within Vb
from the Fermi energy, UðzÞ the local work function, R0an
estimate of the tip curvature radius, and k¼ ﬃﬃﬃﬃﬃﬃﬃﬃ2me
=h: The constant value is set to the value of this expression at an arbitrary point laterally, in the present case at the centre of the cell, and vertically at the height z where the projected density is equal to 10-6electrons/A˚3, with R0= 2 A˚ .
3 Assessment of the computational setup
Atomic basis sets, pseudopotentials and the employed density functional are the most important parameters for the model used in the nanomesh calculations. Basis sets and pseudopotentials have to be chosen carefully to find a balance between accuracy, transferability and computa-tional efficiency. The largest systems will have a size of several thousand atoms and tens of thousands of electrons, and any justified reduction in the basis and the number of explicitly treated electrons will result in huge gains in computer time.
The Gaussian basis sets chosen for this type of appli-cation are of the molecularly optimized type  (Molopt basis). These basis sets are generally contracted and have a single set of exponents for all angular quantum numbers (family basis). The full contraction avoids single functions of diffuse character and results in well-conditioned overlap matrices for all kinds of systems. The basis sets include 4 primitives (B), 5 primitives (N), 6 primitives (Cu, Ni, and Rh), and 7 or 6 primitives (Ru) of s, p, d, and f type functions. The primitives are contracted to a small number of basis functions, and we denote the basis sets with [n|ijkl], where i, j, k, and l are the number of contractions of the s, p, d, and f type and n is the number of primitives. The exponents and contraction coefficients have been globally optimized with respect to the total energy of a small set of reference molecules. The basis sets used are for B [4|221], N [5|221], Cu [6|2221], and Ni [6|3221]. For Rh, either the [6|212] and [6|2221] basis sets with the large core pseudopotential (9 electrons, q9) or the [6|3221] basis with 17 electrons (q17) are employed; for Ru, either the [6|212] basis with 8 electrons (q8) or the [7|3221] with the q16 pseudopotential (q16).
Core electrons are described by dual-space pseudopo-tentials [36–38]. The potentials have been optimized in atomic calculations using the PBE [39,40] functional. It is expected that the potentials perform equally well for the closely related revised PBE  functional.
In order to assess the computational setup, we calculated a series of properties of bulk metals and corresponding rel-evant surfaces and compared them with experiments and published DFT results. Table1shows results for the lattice constants calculated for the four metals considered. Results for the revised PBE functional and our chosen basis sets and pseudopotentials are compared to PW calculations with the same pseudopotentials (‘‘PW-PP’’) [47–49], PW calculations using the projector-augmented wave (PAW) method  using the Quantum ESPRESSO code , and the experimental value. The effect of adding the empirical vdW corrections to the DFT energy is also shown.
With the revPBE functional, the optimized lattice con-stants are consistently larger than with the PBE functional. When either of the empirical vdW potentials is added, the lattice constants become smaller, as expected. The Molopt basis set calculations usually result in slightly smaller lat-tice constants when compared to PW calculations using the same pseudopotential. The only exception is Rh where we find a larger value. The contraction induced by the vdW potentials is typically 1.5 % and slightly larger for the D2 than for the D3 correction. However, in copper the effect is reversed. The final lattice constant calculated with GPW
and the revPBE?D3 functional is very close to the experimental value for Rh and Ru, whereas it is about 2 % too small for Cu and Ni.
Further evidence of the performance of the model setup is shown in Table2 where the bulk modulus, surface energy, and work function are reported. We consider the (111) surface for the three fcc metals (Ni, Cu, and Rh), and the (0001) surface for the hexagonal Ru lattice. The achieved accuracy is comparable in all four TMs.
As we are interested in very large systems and the prop-erties of the metal support are often only of minor concern, we have also investigated the performance of pseudopotentials with fewer valence electrons for Ru and Rh. This basis set/ pseudopotential setup is particularly interesting for the study of molecules interacting with the nanomesh. In these cases, we can trade in a slightly reduced accuracy in the description of the metal surface for an increased computational perfor-mance. However, as we are dealing with a large metallic system, the computational cost is dominated by the diago-nalization of the Kohn–Sham matrix.
Even when not the entire eigenvalue spectrum is needed, the computational cost will scale cubically with the total number of basis functions. Hence, simply reducing the number of explicitly treated electrons by changing the pseudopotential is unlikely to improve performance sig-nificantly. Smaller basis sets also have to be used together with the q8 pseudopotential for Ru and the q9 pseudopo-tential for Rh. The new setup for Ru is [6|212] with the q8 pseudopotential and the two new setups for Rh [6|2221] or [6|212] together with the q9 pseudopotential.
Table3 compares the lattice constant, bulk modulus, surface energy, and work function obtained for Ru and Rh using the small valence setups and the ‘‘reduced size’’
setups. For this comparison, the revPBE?D2 approach has been selected. The results are in reasonably good agree-ment, thus validating the use of ‘‘reduced size’’ setups for Table 1 Optimized lattice
constants [A˚ ]
GPW calculations use 8 9 8 9 8 unit cells. PW-PP and PW-PAW calculations involve one unit cell and are converged with respect to k-points and PW cutoff. Optimizations for Ru used a constant c/a ratio
PBE revPBE revPBE?D2 revPBE?D3 Experiments Ni q18 [6|3221] 3.479 3.501 3.429 3.440 3.5171  PW-PP 3.522 3.548 3.465 PW-PAW 3.520 3.546 3.465 Cu q11 [6|2221] 3.620 3.640 3.558 3.539 3.6149  PW-PP 3.648 3.673 3.584 PW-PAW 3.644 3.676 3.589 Ru q16 [7|3221] a 2.718 2.730 2.685 2.700 2.7059  c 4.292 4.311 4.240 4.265 4.2815  PW-PP a 2.759 2.769 c 4.366 4.382 Rh q17 [6|3221] 3.847 3.864 3.796 3.804 3.803  PW-PP 3.834 3.851 3.781 q9 PW-PP 3.860 3.869 3.802 PW-PAW 3.843 3.854 3.785
Table 2 Bulk modulus B [GPa], surface energy U [eV/A˚2], and work function U [eV] in the studied metal system
Method Functional Cell B / U Ni GPW revPBE exp. 227 0.082 4.83 revPBE?D3 exp. 285 0.165 4.81 PW-PP revPBE exp. 0.106 4.87 PW-PAW revPBE exp. 0.109 4.92 revPBE?D2 exp. 0.174 4.90 exp 186 0.149, 0.153 5.35 Cu GPW revPBE exp. 149 0.073 4.68 revPBE?D3 exp. 203 0.136 4.69 PW-PAW revPBE exp. 0.068 4.81 revPBE?D2 exp. 0.126 4.80 exp 137 0.112, 0.114 4.98, 4.92 Ru GPW revPBE opt. 307 revPBE?D2 opt. 323 0.225 5.01 revPBE?D3 opt. 345 exp 311 0.190 4.47 Rh GPW revPBE opt. 235 revPBE?D2 opt. 250 0.178 5.13 revPBE?D3 opt. 267 5.12 PW-PAW revPBE opt. 238 0.124 5.01 revPBE?D2 opt. 256 0.206 5.02 exp 270 0.166, 0.169 5.0
The experimental values (B from Ref.  except Ru , / from Ref.  and U from Ref. ) are shown in brackets. Computational parameters are the same used for the optimization of the lattice constants reported in Table1
the calculations of the h-BN/TM interfaces, with significant improvements in the computational performance.
3.2 Hexagonal boron nitride
To test the basis sets and pseudopotentials for the elements B and N, we calculated properties of bulk h-BN. These systems also provide insight into the performance of the empirical vdW correction to the density functional for weak interactions. Results are shown in Table4 for h-BN with AA0 and AB stacking. The AA0 stacking contains alternating N and B atoms along the direction perpendic-ular to the BN hexagonal plane. In the AB stacking, the second layer is shifted by a third of the unit cell along the in-plane (11) direction.
The dispersion correction is essential to obtain good agreement with experiment for the interlayer distance because the GGA functionals do not describe the vdW interactions. In particular, both variations of the Grimme potential (D2 and D3) give a slightly too short interlayer separation between the hexagonal BN planes, while the calculated bond lengths are not affected by the dispersion correction and agree well with experiment and previous theoretical estimates.
4 h-BN/metal interface
Thermal decomposition of borazine on hot TM surfaces can lead to the formation of a Moire´ lattice of a highly regular and corrugated h-BN monolayer on the hexagonal metallic surface (for the fcc metals (111) and for Ru the hcp(0001) orientation). The periodicity of such super-structures at the h-BN/metal interface depends strongly on the lattice constant mismatch between h-BN and metal, but can also be influenced by the preparation details . We investigate four systems: two where the lattice constant mismatch is almost 10 % and the h-BN overlayer is strongly corrugated (Rh, Ru), forming the so-called nano-mesh , and two with small mismatch and practically no corrugation (Ni, Cu). These systems have previously been investigated using different simulation methods and mod-els. Structures and bonding of h-BN/Rh(111) and h-BN/ Ru(0001) were studied in detail by applying LAPW models [22,24]. The h-BN/Ni(111) system has attracted attention due to the surface magnetization [20,21,25,26], which is retained after h-BN growth. Results on the h-BN/Cu(111) systems have been reported within an extended study on several TMs . More theoretical work on these systems is available in the context of additional molecular inter-actions (water on h-BN/Rh(111) [64,65], metal atoms on h-BN/Rh(111) [27, 66], hydrogen adsorption and interca-lation [18,67]), and in direct connection with experiments [2,5,10,19,23,68].
The mismatch between h-BN and metal is a fundamental parameter that determines binding and corrugation of the h-BN monolayer. For this reason, we choose the size of the simulation cell that reproduces exactly the experimental mismatch using as reference value the equilibrium lattice constant of h-BN as obtained with our setup, i.e., 2.517 A˚ . This results in an effective lattice constant a of 3.801 A˚ for Rh, 3.628 A˚ for Cu, 3.543 A˚ for Ni, and 2.724 A˚ for Ru. Structural optimizations are typically started from a flat Table 3 Properties of Ru and Rh calculated with different basis sets
and pseudopotentials using the revPBE?D2 approach
a B / U Ru q16 [7|3221] 2.685 323 0.225 5.01 q8 [6|212] 2.718 320 0.218 5.00 Rh q17 [6|3221] 3.796 250 0.178 5.13 q9 [6|2221] 3.813 250 0.172 5.14 q9 [6|212] 3.836 234 0.167 5.20 Lattice constant a [A˚ ], bulk modulus B [GPa], surface energy / [eV/ A˚2], and work function U [eV]. The lattice constant of Ru is calcu-lated at a fixed c/a value
Table 4 Crystal properties of the bulk h-BN at two different stackings, AA0and AB, with either no dispersion correction or DFT-D2  and DFT-D3  formalisms
The polymorphs are
energetically degenerate within 1 meV. Cell parameter a, interlayer distance dlayers, and B–N bond distance dB–N[A˚ ]. Other DFT calculations (with PW formalism with the LDA XC functional) and
experimental results are shown for comparison
GPW: revPBE PAW: revPBE PW-LDA Experiments
DFT DFT-D2 DFT-D3 DFT DFT-D2  h-BN: (AA0)
a 2.516 2.512 2.511 2.521 2.515 2.486 2.50  dlayers 4.145 3.154 3.224 5.262 3.076 3.219 3.33  dB-N 1.453 1.450 1.450 1.455 1.452 1.435 1.44 
GPW: revPBE PAW: revPBE PW-LDA Experiments
DFT DFT-D2 DFT-D3 DFT DFT-D2  h-BN: (AB)
a 2.516 2.511 2.510 2.521 2.514 2.478
dlayers 4.148 3.135 3.199 5.318 3.041 3.279
h-BN terminating a slab of four or seven metallic layers and are stopped when the largest gradient is smaller than 4 9 10-4 Hartree/Bohr. The revPBE-GGA is used as the exchange-correlation functional and is augmented with the empirical DFT-D3 dispersion correction unless otherwise stated.
4.1 h-BN adsorbed on Rh(111)
Full models of the h-BN/Rh(111) unit cell have been studied previously [22, 24, 27]. In this section, we will extend our results  and compare them to other studies. The lattice mismatch between h-BN and Rh(111) is quite large, the (111) lattice constant of Rh being -7.0 % larger than that of h-BN. Such a mismatch does not allow a commensurate growth of the overlayer. Instead, a super-structure constituted of 13 9 13 h-BN units on a 12 9 12 Rh(111) surface has been observed. In principle, only a slight distortion of the B-N bond length would be required to match with a flat 13 9 13 h-BN layer on top of the 12 9 12 Rh(111) units. This is an overall contraction of the bonds by 1.4 % from 1.45 to 1.43 A˚ and corresponds to an energy increase of 0.02 eV per BN pair. This has to be compared with a stretching energy of 0.40 eV/BN for the 1 9 1 commensurate structure. In fact, the adsorbed h-BN layer is corrugated, in order to optimize the BN-Rh binding over a larger area. The extent of this area depends on the registry of h-BN over the Rh(111) surface.
4.1.1 Quasi-commensurate adsorption of h-BN on Rh(111) To gain a deeper insight into how the registry affects the binding properties, we first investigate models of smaller size, where the one to one commensurate structure is obtained by stretching the h-BN overlayer. In these models, we use a Rh(111) slab of seven layers and 6 9 6 lateral unit cells. The slab with the q17 pseudopotential for Rh is terminated on both sides with the stretched 6 9 6 h-BN layer to match the lattice constant 3.801 A˚ of Rh. The h-BN layer can be arranged with nitrogen on top of a Rh atom and B on the next hollow site, namely the (N-top,B-fcc) and (N-top,B-hcp) registries, or with nitrogen occupying a hollow site, giving rise to the possible (N-fcc,B-top), (N-hcp,B-top), (N-fcc,B-hcp), or (N-hcp,B-fcc) registries. These test systems are well suited to investigate the importance of the dispersion energy since they act as models for the different bonding situations in the full system. The registries with N atop are the most stable structures, whereas when N occupies a hollow site, the binding is weaker and lateral movement has to be con-strained in geometry optimizations to keep the overlayer in such a position. In Table5, interaction energy, work function, as well as some structural properties are
summarized for the four investigated commensurate 1 9 1 models.
The stretched overlayer remains overall flat in all the registries, even though the B–N bond buckles. The most stable structure is the (N-top,B-fcc) registry, with a mini-mum N-Rh distance of about 2.18 A˚ . The (N-top,B-hcp) is very similar, only 0.034 eV/BN less stable than the (N-top,B-fcc) registry. Since the energy cost for a 1-to-1 matching of h-BN on Rh(111) is quite large, the adsorption energy is only about -0.14 eV per BN pair in the N-top structures, while it is positive in all the N-hollow models. In the latter case, the weak binding is not sufficient to compensate the energy cost for the distortion of the h-BN layer. When N occupies hollow sites, the vertical distance from Rh(111) increases and the buckling is reduced. The buckling can be explained considering the weakened B–N bond, due to the stretching of the h-BN layer and a partial charge redistribution. Indeed, due to the presence of the metal, the electronic charge localized around the N atoms is polarized towards the Rh slab. Hence, the positively charged B atoms get attracted towards the negatively charged interlayer region. This effect is more evident in the N-top registry, where the N-Rh interactions and the polarization of N-pzelectrons are stronger. In this case, we
can consider the N-p band as hybridized with the metal d band.
In order to characterize the electronic structure, we make use of the MLWFs. The displacements of the centres of charge, or Wannier centres (WC) of the MLWFs, with respect to the nuclear cores in different chemical envi-ronments can be used as an indicator of polarization. In free-standing h-BN, three such WCs are found along the three in-plane B–N bonds of each nitrogen atom. The fourth centre, representing the nitrogen lone pair, is located at the N atom. In the N-top structure, instead, the lone-pair WC is displaced into the interlayer region, indicating a polarization of the electronic charge distribution due to the interaction with the metal. As a consequence, the work function of the system is reduced from 5.01 eV of bare Rh(111) to 3.07 eV. Such N–Rh binding interaction is not observed in the N-hollow configurations, and the lone-pair WC is located within the h-BN plane like in the Table 5 Properties of the quasi-commensurate h-BN/Rh(111) sys-tem, using the symmetric slab model at the four registries: Interaction energies [eV/BN], work function U [eV], and distances and buckling [A˚ ]
N B Eint U dmin(N) bB–N
top fcc -0.621 3.07 2.184 0.139
top hcp -0.587 3.07 2.193 0.141
fcc top -0.323 3.83 2.590 0.088
free-standing h-BN. The work function in this case is 3.8 eV, almost independent of the specific registry.
In the (N-top,B-fcc) and (B-top,N-fcc) models, we have investigated the effect of the empirical dispersion correc-tion term and the basis set superposicorrec-tion error (BSSE). The counterpoise correction method results in a 3 % correction, or destabilisation, of the interaction energy in both cases. The interaction energy computed in the two models as function of the distance of the h-BN layer from the surface is displayed in Fig.1. In these calculations, the structure has not been relaxed. In the case of strong interaction (N-top), DFT(revPBE) alone results in bonding at distances between 2.1 and 2.5 A˚ , with a minimum at about 2.3 A˚. This bonding is slightly enhanced by the dispersion cor-rection, which results in a decrease in the equilibrium distance. In contrast, the weakly bound system has all its binding energy from the dispersion contribution. The effect of the actual type of dispersion correction used (D2 vs. D3) is minor, the D3 correction always being slightly weaker than the D2 correction. In the full nanomesh, the dispersion forces play an important role in the weakly bound region (wire). The effect is that the wire lies closer to the metal surface, thus reducing the overall corrugation. The same effect has been seen in graphene systems .
4.1.2 h-BN/Rh(111) nanomesh
The full supercell for the nanomesh is constructed with the metallic slab of 12 9 12 lateral unit cells of Rh(111) ter-minated with a 13 9 13 h-BN overlayer. We tested several different models by changing the thickness of the slab, from four to seven layers, and pseudopotential and basis set of Rh, i.e., both q17 and q9 pseudopotentials with the
[6|3221] and [6|212] basis sets, respectively. For B and N, we always use q3 and q5 pseudopotentials and [4|221] and [5|221] basis sets. The largest tested model is a symmetric slab of 7 layers (1008 Rh atoms) and one h-BN overlayer per side (338 BN pairs), for a total of 1,684 atoms. With the q17 pseudopotential and the largest [6|3221] basis set for Rh, this amounts to 19,840 electrons and 34,996 basis functions. Nevertheless, similar structural and electronic properties of the nanomesh are obtained with the compu-tationally more convenient setup employing q9 pseudopo-tential and [6|212] basis set. In what follows, we report the results for the seven layer slab with h-BN on one side only (non-symmetric system) and the bottom-most layer is kept fixed with the atoms in bulk positions. With this model, we allow the relaxation of the metal layers deeper inside the slab. This is important in order to be able to estimate how much the interaction with h-BN affects the substrate.
Upon starting the optimization of the full system with a flat and contracted h-BN overlayer (1.4 % contraction of B–N bond length), it slowly adjusts to the substrate, building up a corrugation pattern and modulation of the B–N bond length. From the height colour map in Fig.2a), where the B and N atoms are coloured in red (pore) and blue (wire), two flat regions are clearly identified. The pore region contains the atoms that are closer to the metal (2.2–2.4 A˚ ). Here, the registry is approximately (N-top,B-fcc) and the B–N bond length tends to be stretched with respect to free-standing h-BN (see Fig.2b), in order to maximize the N–Rh contact and thus the pore area. For the same reason, Rh atoms below the pore have a slightly shorter Rh–Rh bond distance of 2.67 A˚ . The shape of the pore is approximately hexagonal and it is centred on three on top N atoms. The wire region lies about 1 A˚ higher, between 3.2 and 3.4 A˚ . Here, the B atoms are approxi-mately on top and the bond length is contracted. The steep change in height involves only two BN rows (yellow and green in the figure). The pore region corresponds to about 20 % of the overlayer. The wire involves slightly more than 50 % of the area. The adsorption energy Eadsper BN
pair is calculated to be -0.25 eV. This value contains the energy loss due to the contraction of the flat h-BN layer, 0.02 eV/BN, the energy loss due to the corrugation of the contracted overlayer, 0.03 eV/BN, and the energy loss due to the corrugation of the Rh layers, induced by the inter-action with h-BN. The bare interinter-action energy between h-BN and metal amounts to -0.31 eV/BN.
The hybridization of the N lone pairs with the Rh d band is responsible for the bonding interaction in the pore region. The charge density difference map reported in Fig.3 shows that modifications of the charge distribution due to the interaction between h-BN and Rh are visible only in the region of the pore. In the region between the metal surface and h-BN, accumulation of charge is
2.0 2.5 3.0
Vertical Distance BN-Rh top layer [Å] -0.80 -0.60 -0.40 -0.20 0.00 0.20 0.40 0.60 0.80 Energy [eV] 2.5 3.0 3.5-0.80 -0.60 -0.40 -0.20 0.00 0.20 0.40 0.60 0.80 revPBE D2 D3 revPBE+D2 revPBE+D3 N-top, B-fcc B-top, N-fcc
Fig. 1 Interaction energy as a function of the vertical displacement of the h-BN overlayer calculated in the h-BN/Rh(111) system: DFT(rev-PBE) contribution (red), and the contribution of only the dispersion D2 (blue) and D3 (green). The total potential energy can be obtained by summing red and blue (revPBE?D2, blue dashed) or red and green (revPBE?D3, green dashed) lines
observed at the first Rh layer (red iso-surface at ?0.005 e/A˚3 and red areas in the volume slice). The displaced charge comes mainly from the N atoms and from the first layer of Rh atoms, where depletion areas (black iso-surface) are visible. The blue areas in the volume slice in Fig.3b indicate that charge is subtracted from the area around the N, whereas red areas are in the interlayer region under both N and B. All other parts of the metal as well as the wire region of the nanomesh do not show any charge redistribution. The description of the charge distribution via Mulliken atomic charges shows that N atoms turn out to be less negative than in the free-standing h-BN, while B atoms tend to keep their positive charge. Overall, the h-BN layer is partially positive and the missing negative charge is located at the slab sur-face, below the pore.
In Fig.4a, the simulated STM topography, obtained at a bias potential of -1 eV with the method described in Sect. 2, is reported. The iso-current surface has been generated
starting with a value of isodensity nb= 10-6 e/A˚3; it lies
about 3 A˚ above the h-BN overlayer. The overall corru-gation of this topography map is about 1 A˚ , as also shown by the height-profile obtained along the black-dashed line crossing through the centre of the pore region. The vertical position of the WCs can be used to show the correlation of amount of bonding with the distance of the overlayer from the metal surface. In Fig. 4b, the distance along the z axis of each lone-pair WC from the closest N atom is reported on the ordinate, while on the abscissa is the height of the corresponding N atom above the Rh surface. In this plot, the height-to-polarization correlation is clearly visible. In particular, we notice that in the presence of the Rh(111) substrate, the WC-N distance increases when the N is closer to the metal (red squares). This effect is not visible in the corrugated free-standing h-BN (green squares), where the lone-pair WCs remain at about 0.2 A˚ from N, irrespective of the height of N. The charge density
Vertical distance N-Rh top layer [Å]
1.453 1.432 BN bond-length [Å] 1.47 1.46 1.45 1.44 1.43 2 2.5 3 3.5 (b) (a) Fig. 2 aHeight colour map of
the B and N atoms, measured relative to the average height of the topmost Rh layer, in the h-BN/Rh(111) nanomesh. The height ranges for each colour are given in the legend of the figure. The small grey spheres represent the Rh atoms of the slab underneath. b B–N bond length versus the height of the N atoms over the topmost Rh layer. The green and red horizontal lines indicate the equilibrium B–N bond length and the bond length of flat 13 9 13 h-BN over the 12 9 12 Rh(111) units, respectively (a) (c) (b) Rh-1 Rh-3 Rh-4 Rh-7 N B Rh-6
Fig. 3 aTop view of the charge density difference in the h-BN/ Rh(111) nanomesh. The red and the black iso-surfaces in the top view indicate a difference of ?0.005 and of -0.005 e/A˚3, respectively. b, c Slice cutting through the middle of the pore through N and B atoms, respectively. The range of the colour map from blue to red corresponds to values from -0.005 to ?0.005 e/A˚3
polarization in the pore region directly leads to a strong modulation of the electrostatic potential and, consequently, of the local work function. Figure4c contains the map of the local work function over the simulated STM iso-current surface displayed in panel a). The resulting work function map can be compared to experimental dI/dz maps . Along the line crossing diagonally through the pore, we estimate a difference in work function between wire and pore of about 0.45 eV. It is this strong change in electro-static potential that is responsible for the trapping of mol-ecules and atoms in the pore .
4.2 h-BN adsorbed on Ru(0001)
The a parameter of the Ru hexagonal lattice is 8.2 % larger than that of h-BN. Hence, it is reasonable to expect that similar structures as those observed on Rh(111) can be formed on the Ru(0001) surface. Indeed, the formation of a nanomesh of h-BN on Ru(0001) was reported first in 2007 . The periodicity of 13-on-12 was considered to be the most likely  and was therefore subsequently used in the theoretical studies by Laskowski and Blaha  and Wang and Bocquet . Comparison with experiments also supported this periodicity, as h-BN deposited on thin Rh(111)-films grown on yttrium-stabilized zirconia on Si(111)  resulted in a 14-on-13 structure: It was argued that the slightly smaller lattice constant of the Rh-film compared to bulk Rh(111) and the slightly different ther-mal expansion coefficients are responsible for the forma-tion of this larger superstructure. Extrapolating this line of argument to a Ru(0001) single crystal, it was predicted that either a 12-on-11 or a 13-on-12 nanomesh superstructure would be formed at the growth temperature of 900 K.
However, using surface X-ray diffraction , a 14-on-13 structure was found. According to the proposed interpre-tation, energy minimization from the stronger bonding of h-BN to Ru in comparison with h-BN/Rh(111) overcomes the increased strain energy and leads to the formation of a larger superstructure, 14-on-13, rather than the smaller 13-on-12.
Here, we consider both the proposed superstructures for h-BN on Ru(0001), i.e., the 13-on-12 and the 14-on-13, and compare to the 13-on-12 h-BN on Rh(111) nanomesh. In these calculations, we employ the q8 pseudopotential and the [6|212] basis set for Ru. The models contain seven Ru layers terminated by the h-BN overlayer on one side only. On the opposite side of the slab, the Ru atoms of the ter-minating layer are fixed at bulk positions. The flat 13 9 13 h-BN overlayer can match the 12 9 12 Ru(0001) surface without distortion, whereas in the 14-on-13 superstructure, the B-N bond length has to be elongated by 0.5 %. How-ever, as observed already on Rh(111), starting the optimi-zation from a flat overlayer, a strongly corrugated structure is formed in both registries, where lower and higher regions correspond to elongated and contracted B–N bonds, respectively. The 14-on-13 superstructure turns out to be energetically favoured, with an adsorption energy 0.012 eV/BN lower than that of the 13-on-12. The reason is the larger low and flat region (pore) with approximately (N-top,B-fcc) registry, where the N–Ru interaction is maximized. On Ru, the corrugation is more pronounced than on Rh, being about 1.7 A˚ in 13-on-12 and 1.5 A˚ in 14-on-13 models. The height colour map of the 14-on-13 structure is reported in Fig.5a. The area of the wire region (blue) is substantially smaller compared to the nanomesh on Rh, indicating a better contact between the overlayer
10 30 50 20 40 4.2 4.1 4.0 3.9 4.3 x axis [Å] 20 40
(b)N height [Å] 2 2.5 3 0.1 0.2 0.3 0.5 0.6 0.4 WC-N vertical distance [Å] hBN/Rh (111) corrugated BN 4.1 3.9 4.3 [eV] [Å] 10 30 50 20 40 6.2 5.8 5.4 20 40 x axis [Å] 6.6 6.0 5.4
Fig. 4 a Simulated STM Tersoff-Hamann iso-current surface obtained at a bias potential of -1 eV at the h-BN/Rh(111) nanomesh. The axis units are A˚ . b Absolute vertical distance of the lone-pair WC from N versus height of N at the nanomesh (red) and at the corrugated
but free-standing h-BN with the same coordinates as in the full system (green). c Modulation of the local work function calculated at the Tersoff-Hamann iso-current surface. The values of the work function are in eV
and the TM in the present case. In the pore, the B–N bond length is elongated in order to optimize the (N-top,B-fcc) registry, with bonds as long as 1.52 A˚ . The overlayer keeps a good contact with the substrate even at the outer ring of the pore region, where the N atoms are displaced from the top sites. Hence, the interaction area on Ru(0001) is more extended, including also the region of the overlayer where the B–N bond is located above Ru, with approximately bridge-type registry. This is clearly visible in the charge density difference map reported in Fig.6. The charge redistribution affects more than 50 % of the overlayer. Electronic charge is displaced from the N lone pairs and the B–N bonds (black iso-surface) towards the metal, thus creating an accumulation of charge in the interlayer region (red iso-surface). Moreover, the footprint of the h-BN–Ru interaction extends deeper into the metallic slab than what is observed in the Rh(111) system, namely the plane cut-ting through the pore (panels b and c in Fig.6) shows
significant charge redistribution between the second and third Ru layers. Also the corrugation of the metallic layers below the nanomesh is larger than in Rh (cf. data in Table6). Due to the more effective interaction, even if the stronger corrugation causes larger energy loss, i.e., 0.14 eV/BN in the 14-on-13, the adsorption energy on Ru(0001) is more than 0.1 eV per BN pair lower than on Rh(111).
The nature of the electronic interaction between Ru and the overlayer can be better understood from the PDOS. Figure7 displays the PDOS on N and B p-states, distin-guishing between the contributions from the atoms belonging to the pore region and those in the wire region. The interaction with the metal mostly affects the occupied p-states on the pore N. The corresponding band shifts to lower energy due to the hybridization with the Ru d band. On the contrary, the B PDOS show much smaller changes between pore and wire, suggesting that B is less directly involved in the orbital re-hybridization.
BN bond-length [Å]
2 2.5 3 3.5
Vertical distance N-Ru top layer [Å]
(a) Fig. 5 aHeight colour map of
the B and N atoms, as measured relative to the average height of the topmost Ru layer in the optimized 14-on-13 h-BN/Ru structure. The height ranges for each colour are given in the legend. The small grey spheres represent the Ru atoms of the slab underneath. b B–N bond length versus the height of the N atoms above the topmost Ru layer. The green and red horizontal lines indicate the equilibrium B–N bond length and the bond length of flat 14 9 14 h-BN over the 13 9 13 Ru(0001) units (a) (c) (b) Ru-1 Ru-3 Ru-5 Ru-7 Ru-2 Ru-4 Ru-6 N B
Fig. 6 aTop view of the charge density difference in the 14-on-13 h-BN/Ru nanomesh. The red and the black iso-surfaces in the top view indicate a difference of ?0.005 and of -0.005 e/A˚3, respectively. b, c Plane cutting in the centre of the pore through N and through B, respectively. The range of the colour map from blue to red corresponds to values from -0.005 to ?0.005 e/A˚3
4.3 h-BN adsorbed on Cu(111)
Compared with other metal substrates, copper has so far received little attention for h-BN adsorption. An experi-mental study using XAS and photoemission spectroscopy  revealed only weak chemisorption of h-BN on Cu(111) and a very flat layer. More recently, Laskowski et al.  included Cu in a systematic theoretical study of TM sub-strates for h-BN. They used the LAPW method to study 7-layer metal slabs with a commensurate 1 9 1 registry. They report results obtained with different XC functionals, LDA, PBE, and Wu-Cohen-GGA (WC-GGA) . The LDA interaction energy is -190 meV/BN for h-BN adsorbed in the (N-top,B-fcc) registry, the height over the Cu(111) surface 3.10 A˚ , and the B-N buckling 0.02 A˚. On the other hand, Eint is only -10 meV/BN with the
WC-GGA functional and the monolayer turns out to be unbound (positive Eint) with PBE. We note that no dispersion
cor-rection was applied in these calculations.
In this work, the previously discussed setup is employed to determine adsorption energies and structural properties of the h-BN/Cu system with six different registries. The Cu(111) slab of seven 6 9 6 layers is symmetrically ter-minated on both sides by a 6 9 6 h-BN layer, located at an initial vertical distance of 2 A˚ . The h-BN and Cu lattices match quite closely, with h-BN having a 2.2 % smaller in-plane lattice parameter. In order to match the Cu(111) lattice, the h-BN layer is thus stretched, thereby elongating the bond lengths by the 2.2 %. Upon the optimization, the B–N bond length is not exactly uniform over the layer anymore and these adjustments cause a minute offset with respect to the assigned registry and the observed small corrugation (\0.03 A˚ ). Adsorption and interaction energies as well as some structural parameters from all the six structural optimizations are listed in Table 7.
As can be seen from both the adsorption energies and the h-BN-metal separation, the differences among the registries are quite small. Eads is always negative (i.e.
binding) and very close to Eint, which is about 30–50 meV
smaller, except in (N-top,B-hcp) where the two energies are essentially equal. This is an indication that the mono-layer remains largely unchanged upon adsorption, i.e., effective interaction is weak. The work function, U; spans a range of 0.1 eV from 3.62 to 3.71 eV. The systems are also similar in geometrical structure. In all registries, the adsorbate layer is approximately 3 A˚ (2.99–3.03 A˚) from the metal surface and is very flat, as indicated by the small h-BN corrugation.
In contrast to previous studies, our work explicitly takes into account dispersion contributions to the adsorption Table 6 Summary and comparison of results for h-BN on Rh(111)
and Ru(0001) h-BN/Rh 13-on-12 h-BN/Ru 13-on-12 h-BN/Ru 14-on-13 EBNdist 0.022 0.0001 0.004 Eads -0.254 -0.367 -0.380 Eint -0.310 -0.520 -0.542 EBNcorr 0.032 0.134 0.139 dmin(N) 2.208 2.186 2.186 dmin(B) 2.128 2.082 2.076 DhN 1.082 1.665 1.497 DhB 1.175 1.754 1.640 Dh1stTM 0.153 0.258 0.247 Dh2ndTM 0.157 0.248 0.256 Dh3rdTM 0.125 0.202 0.212 DhSTM 1.0 1.7 1.6 DU 0.5 0.36 0.35 pore % (\2.4 on Rh; \2.2 on Ru) 20 43 46 wire % ([3.2 on Rh; [3.3 on Ru) 52 23 19
Energies are given in eV/BN, distances and corrugations in A˚ , work functions in eV. EBNdist is the distortion energy of the flat free-standing h-BN, Eadsthe adsorption energy, Eintthe interaction energy, and EBNcorr the corrugation energy of the distorted free-standing h-BN. dmin(N), dmin(B), and DhB;Nare defined in the text. DhTMof the first three TM layers is computed as the difference between minimum and maximum height of the metal atoms within each corresponding layer. The corrugation of the simulated STM topography, DhSTM, is obtained from the iso-current surface at a bias of -1 eV, and the modulation of the local work function DU is computed at this same iso-current surface
-15 -9 -3 3 9 -15 -9 -3 3 9
E-Ef [eV] E-Ef [eV]
N-p all pore wire N-px,y N-pz B-px,y B-pz B-p
Fig. 7 PDOS in the 14-on-13 h-BN/Ru(0001) nanomesh on N and B p-states normalized by the number of atoms included in the projection. The PDOS obtained from all the N or B atoms in the overlayer, and only from the atoms in the pore and the wire are shown with black, red, and blue lines, respectively
energies. These appear to be significant in order to obtain a monolayer adsorbed in a stable way, as opposed to the very weakly bound or unbound systems. However, as vdW interactions are unspecific and only attractive, they do not make clear distinction among the various possible regis-tries. Due to a small electronic effect, configurations with N atop turn out to be somewhat energetically favoured to the others, which confirms previous results [20, 21]. However, we cannot confidently distinguish between (N-top,B-fcc) and (N-top,B-hcp). The energetic differences between the remaining four registries are also too small to establish a well-defined hierarchy of stability.
We have investigated the influence of the h-BN–Cu interaction on the electronic structure of the h-BN by comparing the PDOS and the charge density distribution. In general, the observed effects are small, and therefore, we do not show plots of the results here. By mapping the total density differences, only a slight polarization of the monolayer upon adsorption is revealed, largely indepen-dent of the registry. The major difference in the PDOS on the pz states of N between the (N-top,B-fcc) and the
(N-fcc,B-hcp) configurations, the structures with the smallest and largest values of the work function, is a shift of the valence band by about 0.3 eV.
More recently, it has been shown  that the -2.2 % lattice mismatch between Cu(111) and h-BN causes the formation of Moire´ patterns also at this interface, accom-panied by small rotations of the overlayer with rotation angles from 1 to 10 degrees. The resulting superstructures have much larger unit cells and the simulations become much more challenging. Further discussion of this type of h-BN/Cu(111) superstructure, supported by both experi-ments and calculations, is reported in a separate work . 4.4 h-BN adsorbed on Ni(111)
Several theoretical [20,21,23,25,74] and experimental [8, 10,26] studies on the adsorption of h-BN on nickel sur-faces have been published, focusing on various structural,
energetic, and spectroscopic aspects. Among the possible metal substrates, the Ni(111) in-plane lattice constant (2.49 A˚ ) matches that of h-BN most closely, allowing the formation of an almost perfectly commensurate overlayer. Since the earliest experiments of h-BN/Ni [75, 77], the nature of the bonding of the monolayer to the surface has been discussed repeatedly. Some authors have argued for a weak physisorption-like interaction , while others have proposed a strong(er), chemisorption-like binding .
Table8 summarizes a number of previously published studies of this system, both theoretical and experimental. In particular, we list energetic (adsorption energy) and structural (interlayer distances and corrugations) features as well as the change in surface magnetic moment upon monolayer adsorption. A number of different adsorption geometries were considered by varying the registry of h-BN on Ni(111), leading in some cases to a notable var-iation in the obtained results. In general, however, all studies find the most stable adsorption registries to be those with N atop the Ni atoms and B either in the hcp or fcc sites, the latter typically slightly preferred. Furthermore, the h-BN layer tends to be slightly buckled in a way that places the N atoms further from the metal as in the case of Rh and Ru. Another common observation is the large variation in adsorption energies depending on the employed exchange-correlation approximation. For instance, Laskowski et al. report adsorption energies of -0.27, -0.19, and -0.04 eV/BN with LDA, WC-GGA, and PBE, respectively.
We carried out geometry optimizations of h-BN on Ni considering all six possible high-symmetry registries. The Ni(111) slab of seven 6 9 6 layers is symmetrically ter-minated on both sides by a 6 9 6 h-BN layer. Since the lattice constants match quite precisely, no large deforma-tions of the h-BN layer are expected upon optimization. The calculated adsorption energies and work functions, as well as some structural parameters obtained in different registries are summarized in Table 9. The strongest inter-action is obtained when the N atoms are atop surface atoms. In this case also, the distance from the substrate is significantly shorter than in structures where the N is located at the hollow sites. The differences among all other registries are much less pronounced, although when both B and N occupy hollow sites the distance from the substrate is slightly larger, the buckling smaller, and the work function larger. Furthermore, we observe a reduction in the surface magnetic moment from 0.65 to 0.50 lB as
the interlayer distance decreases, the last value being the equilibrium result. Compared to the magnetic moment of the free Ni(111) surface, 0.73 lB, this corresponds to a
reduction of -0.08 to -0.23 lB, in good agreement with
previously published values (cf. Table8). The magnetic moment of the innermost metal layer (bulk-like), however, Table 7 Properties of the commensurate h-BN/Cu(111) system,
using the symmetric slab model in the six registries: adsorption and interaction energies [eV/BN], work function U [eV], and distances, corrugation and buckling [A˚ ]
N B Eads Eint U dmin (B) dmin (N) DhN bBN top fcc -0.270 -0.298 3.62 2.962 2.977 0.010 0.015 top hcp -0.265 -0.262 3.63 2.966 2.980 0.020 0.015 fcc top -0.244 -0.284 3.66 2.959 2.976 0.052 0.016 hcp top -0.229 -0.273 3.67 2.969 2.985 0.043 0.016 fcc hcp -0.234 -0.281 3.71 3.023 3.036 0.006 0.013 hcp fcc -0.234 -0.280 3.69 3.019 3.032 0.045 0.013
remains unchanged with a magnetic moment of about 0.58 lB, irrespective of the monolayer-surface distance.
In the most stable registries, our results agree well with the published experimental values of interlayer distance and corrugation, being between the values determined from LEED and XPD. The distance between h-BN and Ni(111) and the corrugation of the overlayer also agree well with most previous computational studies [20, 21, 74] (cf. Table8). The computed adsorption energies indicate also in the case of Ni(111) that the configurations with N atoms atop the surface Ni atoms are most stable. It is, however, not possible to definitively distinguish between B-fcc and B-hcp due to the very small differences in adsorption energy. h-BN turns out to be chemisorbed on Ni(111) in all six registries, with generally significantly stronger adsorp-tion energies than previous studies have shown. This effect can be attributed to the contribution from the vdW cor-rection, which was not considered in previous studies.
Figure8 contains the spin-polarized PDOS projected on the Ni and N atoms in the most strongly bound registry, (N-top,B-fcc). The left column shows curves in the bulk and the surface atoms of the h-BN/Ni system and those at the bare Ni surface for comparison. The most pronounced change in the PDOS around the Fermi level upon the adsorption of h-BN occurs in the dxz, yzand dz2states, while
the orbitals without a z component remain largely unaf-fected. For all orbitals, we observe a pronounced peak in the spin a channel just below the Fermi level and at or beyond it in the b-PDOS. Upon adsorption, these peaks shift to lower and higher energies in the dz2 and dxz, yz orbitals, respectively.
In the right column of Fig. 8, the electronic states are projected on the N p orbitals. We tried to adjust energy reference of the PDOS from the free-standing to one from the adsorbed h-BN by aligning the low-energy peaks, but when the peaks in the px,ymatch well, in pzthe main peaks
are about 1 eV higher in energy in the free-standing h-BN; this indicates a different response in the two different kinds of p orbitals to the adsorption. Interestingly, the largest peaks more than 3 eV below the Fermi energy in the spin a and b pz PDOS lie at the same energies, differences
appearing only close and above the Fermi energy. Com-pared to a free-standing h-BN sheet, a number of weak gap states appears upon the adsorption, mainly originating from pz. The shape of the curves remains otherwise quite similar,
indicating that the electronic structure of the adsorbate is affected only weakly by the adsorption. We also note a small spin polarization of the PDOS, shifting the b channel to slightly higher energies, and some differences in gap states between the two spins.
Table 8 Adsorption energy [eV/BN], layer separation and corrugation [A˚ ], and change in magnetic moment of the surface Ni atoms [lB] upon adsorption of the h-BN overlayer on Ni(111) at different registries
Method XC Eads dmin(B) bB-N Dlsurfper Ni References
DFT PBE-GGA – 2.08 0.11 -0.08  DFT PW91-GGA -0.021–0.038 2.18 – 3.97 – -0.00 to -0.23  LDA -0.420 to -0.141 1.95 – 3.11 – -0.02 to -0.43  DFT PBE-GGA -0.04 2.04 0.11 -0.06  WC-GGA -0.19 2.03 0.11  LDA -0.27 2.01 0.11  DFT PBE-GGA -0.04 1.99 0.10 – 
DFT revPBE?D3 -0.392 2.008 0.124 -0.08 to -0.23 Present work
LEED – 2.20 0.2 – 
XPD – 1.95 0.07 – 
Table 9 Adsorption and interaction energies [eV/BN], work function U [eV], and distances, corrugation and buckling [A˚ ] in the h-BN/Ni(111) system, using a 6 9 6 symmetric slab model in the six registries listed
N B Eads Eint U dmin(B) dmin(N) DhBN bB-N lsurfper Ni
top fcc -0.390 -0.470 3.58 2.006 2.130 0.001 0.123 0.519 top hcp -0.392 -0.473 3.55 2.008 2.132 0.001 0.124 0.503 fcc top -0.283 -0.257 3.84 2.903 2.921 0.010 0.022 0.635 hcp top -0.283 -0.268 3.84 2.923 2.944 0.057 0.021 0.630 fcc hcp -0.285 -0.269 3.90 3.015 3.028 0.028 0.016 0.651 hcp fcc -0.293 -0.270 3.91 2.996 3.008 0.073 0.016 0.649
Several related investigations of the density of states of h-BN/Ni have been published recently [21,23,74]. Our results are in good agreement with these reports. In par-ticular, our data reproduce the approximate peak shape and position of the Ni dz2 states reported in , both at the
surface with h-BN (3 peaks) and the bare surface (2 peaks). The relative shifts of the peaks closest to the Fermi level upon adsorption are also comparable to those results. Concerning the nitrogen states, the small spin polarization that we find (discussed below) matches the results in Ref. . Che and Cheng  found similar peaks in the N pz
states, only sharper and more pronounced than ours. Complementary to the PDOS plots, maps of the electron and spin density differences are plotted in Fig.9 in the same system. Evidently, the electronic changes upon adsorption are predominantly confined to the h-BN monolayer and the topmost layer of metal atoms, while the lower-lying Ni atoms are largely inert except for a weak polarization in the second layer. The electron density dif-ference indicates a transfer of electrons from the Ni dz2 orbitals to the dxz, yzorbitals and to the interlayer space. At
the same time, the N pz orbitals lose electron density,
whereas the px,y gain some. An opposite effect occurs on
the B atoms, which accumulate electrons in the pzorbitals
and lose some from the in-plane orbitals. The B-pzorbital
gets strongly polarized towards the metal surface. The image also implies a depletion of electrons at the centre of the h-BN honeycomb.
With regard to spin density, the most significant change of magnetism occurs—as expected—in the topmost Ni layer. The spin polarization in the dz2-symmetry orbitals increases, while spin polarization decreases in the dxz,yz
orbitals. Some decrease in spin polarization is also visible in the second Ni layer. More notably, however, the nitrogen atoms are also subject to some magnetic polarization, albeit much smaller in magnitude. In particular, the average magnetic moment (from Mulliken population analysis) of the N atoms is 0.027 lB while that of B is -0.020 lB.
These observations are consistent with the PDOS results discussed above. The upshift of the peak in the
N p h-BN/Ni free h-BN Ni dz2 α β bulk atoms bare surface h-BN/Ni surface N pxy Ni dxy+dx2-y2 -8 -4 0 4 Energy [eV] N pz -8 -4 0 4 Energy [eV] Ni dxz+dyz
Fig. 8 PDOS on Ni d states and N p states in the h-BN/Ni(111) system. States of spin a and b are plotted on the positive and negative vertical axis, respectively. PDOS of a free, non-spin-polarized h-BN sheet is shown for comparison. Plots for Ni show projections on the surface and central atoms of the adsorbate system and of the bare surface for comparison. Energy scale is relative to the Fermi energy, in the free h-BN layer aligned at the peaks in PDOS at deep energies
Fig. 9 Map of the differences upon the adsorption of h-BN in total electron density (left) and spin density (right) of the h-BN/ Ni(111) system. Blue regions indicate depletion of electrons (or magnetic moment), while red areas denote accumulation
dz2-symmetric b PDOS causes the increase in spin polari-zation of the corresponding orbitals, while the move of dxz, yz orbitals to lower energies leads to the loss of spin
polarization in these directions.
In this overview, we have shown that DFT calculations, when carefully set up, can be used to reproduce and explain experimental findings for the nanomesh systems. Our specific approach based on the Gaussian and plane waves method provides a similar accuracy of description as plane wave-based codes. Additionally, we apply a dispersion correction to semi-local density functionals.
The adsorption of h-BN on the various substrates leads to different characteristics of the overlayer structure as summarized in Table10. The strength of the interaction of h-BN with the metals in quasi-commensurate cases—either in real systems of Ni and Cu or in artificial Rh* system when the lattice constant of the overlayer is scaled to match the substrate—follows the expected trend, being larger in the case of the transition metals and weaker on the noble metal Cu. Whether the geometry of the overlayer is flat or buckled is mainly dictated by the lattice mismatch between h-BN and the substrate. On Ru(0001) and Rh(111), the mismatch is large and the interaction in the preferred regions strong. Therefore, an incommensurability is induced that is relieved by forming a corrugated nanomesh, where various lateral registries are found within the unit cell. On the other hand, on Ni(111), the mismatch is very small so that the commensurate (1 9 1) registry is obtained in experiments, with no corrugation. On Cu(111), the interaction is weak and the mismatch small, resulting in Moire´ structures with large periodicities . For all the investigated systems, we have employed dispersion cor-rections to the DFT functional. These corcor-rections are
essential to reproduce reliable structures, in particular when the interaction is weak and the distance between overlayer and substrate is large.
In order to better understand the nature of the interaction between h-BN and the four substrates, we have considered how the electronic structure of the overlayer is modified. On Rh and Ru, the regions where good contact is possible are characterized by strong re-hybridization of the p-states on the N atoms. In particular, we observe that these areas are more extended on Ru, where the 14-on-13 reconstruc-tion turns out to be the most favourable. Like previous studies, our calculations yield the magnetization of the h-BN overlayer on Ni(111). This surface magnetization could lead to applications including spin filtering, as adsorbates on this system would experience a weak, mainly insulating but yet spin-polarized interaction with the h-BN/ Ni(111). Our results confirm that in the spectrum of h-BN– TM electronic interaction strength, Cu resides at the very low end and shows the weakest effects on h-BN of all metals discussed in this study.
Having established reliability and accuracy of the compu-tational method for the overlayer arrangement of h-BN on metal supports, we can go further and use this approach not only to verify and explain experimental findings but also to predict new arrangements and trends of similar nanostructures and for example adsorption and assembly of molecules on them. The first examples have already appeared in the litera-ture: Disappearance of the corrugation in the nanomesh on Rh(111) upon hydrogen intercalation  and water inter-acting with the nanomesh [64,65,68].
Acknowledgments This work is supported by Swiss National Sci-ence Foundation under Grants No. CRSI20 122703 and No. 140441. The authors thank the Swiss National Supercomputer Centre (CSCS) and University of Zurich for generous allocations of computer time. Open Access This article is distributed under the terms of the Creative Commons Attribution License which permits any use, dis-tribution, and reproduction in any medium, provided the original author(s) and the source are credited.
1. Corso M, Auwa¨rter W, Muntwiler M, Tamai A, Greber T, Osterwalder J (2004) Boron nitride nanomesh. Science 303(5655):217–220
2. Berner S, Corso M, Widmer R, Groening O, Laskowski R, Blaha P, Schwarz K, Goriachko A, Over H, Gsell S, Schreck M, Sachdev H, Greber T, Osterwalder J (2007) Boron nitride nano-mesh: functionality from a corrugated monolayer. Angew Chem Int Ed 46(27):5115–5119
3. Goriachko A, He Y, Knapp M, Over H, Corso M, Brugger T, Berner S, Osterwalder J, Greber T (2007) Self-assembly of a hexagonal boron nitride nanomesh on Ru(0001). Langmuir 23(6):2928–2931
Table 10 General properties in the different h-BN/TM and nano-mesh systems: mismatch between the equilibrium hexagonal lattice constants between the h-BN and the substrate [%], corrugation [A˚ ], adsorption energy and interaction energy [eV/BN], smallest vertical TM-N and TM-B distances [A˚ ], and the share of atoms forming the pore region (closer than 2.4 A˚ on Rh and 2.2 A˚ on Ru) [%]
Mismatch DhN Eads Eint dmin(N) dmin(B) In-pore Ni ?0.5 – -0.39 -0.47 2.13 2.07 – Cu -2.2 0.02 -0.27 -0.30 2.98 2.97 – Ru -7.6 1.5 -0.38 -0.54 2.19 2.08 46 Rh -7.0 1.1 -0.25 -0.31 2.21 2.13 20 Rh* 0.0 – – -0.62 2.61 –
Rh*refers to the system where the lattice constant of the h-BN was artificially scaled to match the hexagonal in-plane value of the Rh(111)
4. Preobrajenski AB, Nesterov MA, Ng ML, Vinogradov AS, Martensson N (2007) Monolayer h-BN on lattice-mismatched metal surfaces: on the formation of the nanomesh. Chem Phys Lett 446(1-3):119–123
5. Brugger T, Guenther S, Wang B, Dil JH, Bocquet ML, Osterw-alder J, Wintterlin J, Greber T (2009) Comparison of electronic structure and template function of single-layer graphene and a hexagonal boron nitride nanomesh on Ru(0001). Phys Rev B 79(4):045407
6. Cavar E, Westerstrom R, Mikkelsen A, Lundgren E, Vinogradov AS, Ng ML, Preobrajenski AB, Zakharov AA, Martensson N (2008) A single h-BN layer on Pt(111). Surf Sci 602(9):1722–1726 7. Preobrajenski AB, Vinogradov AS, Ng ML, Cavar E,
Wester-strom R, Mikkelsen A, Lundgren E, Martensson N (2007) Influence of chemical interaction at the lattice-mismatched h-BN/ Rh(111) and h-BN/Pt(111) interfaces on the overlayer morphol-ogy. Phys Rev B 75(24):245412
8. Preobrajenski AB, Vinogradov AS, Martensson N (2005) Monolayer of h-BN chemisorbed on Cu(111) and Ni(111): the role of the transition metal 3d states. Surf Sci 582(1–3):21–30 9. Preobrajenski AB, Krasnikov SA, Vinogradov AS, Ng ML,
Kaambre T, Cafolla AA, Martensson N (2008) Adsorption-induced gap states of h-BN on metal surfaces. Phys Rev B 77(8):085412 10. Shimoyama I, Baba Y, Sekiguchi T, Nath KG (2009) A
theo-retical interpretation of near edge X-ray absorption fine structure of hexagonal boron nitride monolayer on Ni(111). J Electron Spectrosc 175(1–3):6–13
11. Morscher M, Corso M, Greber T, Osterwalder J (2006) Formation of single layer h-BN on Pd(111). Surf Sci 600(16):3280–3284 12. Mu¨ller F, Hu¨fner S, Sachdev H, Laskowski R, Blaha P, Schwarz
K (2010) Epitaxial growth of hexagonal boron nitride on Ag(111). Phys Rev B 82(11):113406
13. Mu¨ller F, Hu¨fner S, Sachdev H (2008) One-dimensional structure of boron nitride on chromium (110)—a study of the growth of boron nitride by chemical vapour deposition of borazine. Surf Sci 602(22):3467–3476
14. Vinogradov NA, Zakharov AA, Ng ML, Mikkelsen A, Lundgren E, Ma˚rtensson N, Preobrajenski AB (2012) One-dimensional corrugation of the h-BN monolayer on Fe(110). Langmuir 28(3):1775–81
15. Allan M, Berner S, Corso M, Greber T, Osterwalder J (2007) Tunable self-assembly of one-dimensional nanostructures with orthogonal directions. Nanoscale Res Lett 2(2):94–99
16. Wintterlin J, Bocquet ML (2009) Graphene on metal surfaces. Surf Sci 603(10–12):1841–1852
17. Dil H, Lobo-Checa J, Laskowski R, Blaha P, Berner S, Osterw-alder J, Greber T (2008) Surface trapping of atoms and molecules with dipole rings. Science 319(5871):1824–1826
18. Brugger T, Ma HF, Iannuzzi M, Berner S, Winkler A, Hutter J, Osterwalder J, Greber T (2010) Nanotexture switching of single-layer hexagonal boron nitride on rhodium by intercalation of hydrogen atoms. Angew Chem Int Ed 49(35):6120–6124 19. Laskowski R, Blaha P, Gallauner T, Schwarz K (2007)
Single-layer model of the hexagonal boron nitride nanomesh on the Rh(111) surface. Phys Rev Lett 98(10):106802
20. Grad G, Blaha P, Schwarz K, Auwa¨rter W, Greber T (2003) Density functional theory investigation of the geometric and spintronic structure of h-BN/Ni(111) in view of photoemission and STM experiments. Phys Rev B 68(8):085404
21. Laskowski R, Blaha P, Schwarz K (2008) Bonding of hexagonal BN to transition metal surfaces: an ab initio density-functional theory study. Phys Rev B 78(4):045,409
22. Laskowski R, Blaha P (2008) Unraveling the structure of the h-BN/Rh(111) nanomesh with ab initio calculations. J Phys Condens Matt 20(6), 2nd workshop on theory meets industry, Erwin Schrodinger Inst, Vienna, Austria, 12–14 Jun 2007
23. Laskowski R, Gallauner T, Blaha P, Schwarz K (2009) Density functional theory simulations of B K and N K NEXAFS spectra of h-BN/transition metal(111) interfaces. J Phys Condens Matt 21(10):104210
24. Laskowski R, Blaha P (2010) Ab initio study of h-BN nanomeshes on Ru(001), Rh(111), and Pt(111). Phys Rev B 81(7):075418 25. Huda MN, Kleinman L (2006) h-BN monolayer adsorption on the
Ni(111) surface: a density functional study. Phys Rev B 74(7):075418 26. Yazyev OV, Pasquarello A (2010) Metal adatoms on graphene and hexagonal boron nitride: towards rational design of self-assembly templates. Phys Rev B 82(4): 045407
27. Wang B, Bocquet ML (2011) Monolayer Graphene and h-BN on metal substrates as versatile templates for metallic nanoclusters. J Phys Chem Lett 2(18):2341–2345
28. Zhou YG, Zu XT, Gao F (2011) Substrate-induced magnetism in BN layer: a first-principles study. Solid State Commun 151(12):883–886 29. Lippert G, Hutter J, Parrinello M (1997) A hybrid Gaussian and plane wave density functional scheme. Mol Phys 92(3):477–487 30. VandeVondele J, Krack M, Mohamed F, Parrinello M, Chassaing T, Hutter J (2005) QUICKSTEP: fast and accurate density functional calculations using a mixed Gaussian and plane waves approach. Comput Phys Commun 167(2):103–128
31. Grimme S (2004) Accurate description of van der Waals com-plexes by density functional theory including empirical correc-tions. J Comput Chem 25(12):1463–1473
32. Grimme S, Antony J, Ehrlich S, Krieg H (2010) A consistent and accurate ab initio parametrization of density functional dispersion correction (DFT-D) for the 94 elements H-Pu. J Chem Phys 132(15):154104
33. Hohenberg P, Kohn W (1964) Inhomogeneous electron gas. Phys Rev 136:B864–B871
34. Kohn W, Sham LJ (1965) Self-consistent equations including exchange and correlation effects. Phys Rev 140:A1133–A1138 35. CP2K (2012) CP2K developers group under the terms of the
GNU General Public Licence; seehttp://www.cp2k.org/
36. Goedecker S, Teter M, Hutter J (1996) Separable dual-space Gaussian pseudopotentials. Phys Rev B 54(3):1703–1710 37. Hartwigsen C, Goedecker S, Hutter J (1998) Relativistic
sepa-rable dual-space Gaussian pseudopotentials from H to Rn. Phys Rev B 58(7):3641–3662
38. Krack M (2005) Pseudopotentials for H to Kr optimized for gradient-corrected exchange-correlation functionals. Theor Chem Acc 114(1-3):145–152
39. Perdew JP, Burke K, Ernzerhof M (1996) Generalized gradient approximation made simple. Phys Rev Lett 77:3865–3868 40. Perdew JP, Burke K, Ernzerhof M (1997) Erratum: generalized
gradient approximation made simple. Phys Rev Lett 78:1396 41. Zhang Y, Yang W (1998) Generalized gradient approximation
made simple. Phys Rev Lett 80:890–891
42. Bendt P, Zunger A (1982) New approach for solving the density-functional self-consistent-field problem. Phys Rev B 26:3114 43. Marzari N, Vanderbilt D (1997) Maximally localized generalized
Wannier functions for composite energy bands. Phys Rev B 56:12847–12865
44. Tersoff J, Hamann DR (1983) Theory and application for the scanning tunnelling microscope. Phys Rev Lett 50:1998–2001 45. Tersoff J, Hamann DR (1985) Theory of the scanning tunnelling
microscope. Phys Rev B 31:805–813
46. VandeVondele J, Hutter J (2007) Gaussian basis sets for accurate calculations on molecular systems in gas and condensed phases. J Chem Phys 127(11):114105
47. Gonze X, Rignanese G, Verstraete M, Beuken J, Pouillon Y, Caracas R, Jollet F, Torrent M, Zerah G, Mikami M, Ghosez P, Veithen M, Raty J, Olevano V, Bruneval F, Reining L, Godby R, Onida G, Hamann D, Allan D (2005) A brief introduction to the ABINIT software package. Z Kristallogr 220(5–6):558–562